Oguchi]. Consequently, we observe a noticeable increase in the relative stability of the MS1 structure for higher-valent metals (in fact, all metal diborides with at least five valence electrons benefit from insertion of an extra metal layer with the largest gain of -340 meV/atom obtained for RhB). However, these electron-rich systems allow other phases with significantly lower energies (prototypes NiAs, NaCl, FeB-b, etc.[@PF]). Hence, we focus on low-electron systems that have been shown to stabilize through incorporation of extra metal layers and could compete with existing phases.

5. Li-B system {#section.Li-B}
==============

[*Overview.*]{} A few compounds at different stoichiometries have been reported for the Li-B system[@PF; @aLi; @bLi; @Alkali; @B-Li; @Li3B14; @LiB3]. On the boron-rich side the experimentally reproducible compounds Li$_3$B$_{14}$ and LiB$_3$ have large unit cells with fractional occupancies[@Li3B14; @LiB3; @PF] and cannot be presently simulated with [*ab initio*]{} methods with desired degree of accuracy. The composition of the most lithium-rich LiB$_y$ compounds (near 50% concentration) apparently depends on synthesis conditions and post-synthesis treatment, as the reported values for $y$ range from 0.8 to 1 (notation explained in Ref. [@xy]). In the early experiments the formed compounds were ascribed compositions Li$_5$B$_4$[@Wan78; @Wan79] or Li$_7$B$_6$[@Dal79]; Wang [*at al.*]{} used a rhombohedral model to explain the observed x-ray patterns[@Wan78; @Li5B4]. However, a more consistent interpretation of the available x-ray data on nearly stoichiometric lithium monoboride has been recently given by Liu [*et al.*]{}[@aLi]. The authors demonstrated that the main x-ray peaks can be indexed with a four-atom hexagonal unit cell $\alpha$-LiB (Fig. 5(a)), which consists of linear chains of boron embedded in hexagonal lithium shells[@aLi].

While the simple $\alpha$-LiB sheds light on what the structure of the lithium monoboride is, an important question remains open as to
Oguchi ]. Consequently, we observe a noticeable increase in the relative constancy of the MS1 social organization for high - valent metals (in fact, all metal diborides with at least five valence electron benefit from insertion of an extra metallic element layer with the largest addition of -340 meV / atom obtained for RhB). However, these electron - rich system allow other phases with significantly lower energies (prototype NiAs, NaCl, FeB - b, etc.[@PF ]). Hence, we focus on low - electron system that have been shown to stabilize through internalization of extra alloy layers and could compete with exist phases. 

 5. Li - B system { # section. Li - B } 
 = = = = = = = = = = = = = = 

 [ * Overview. * ] { } A few compound at different stoichiometries have been reported for the Li - B system[@PF; @aLi; @bLi; @Alkali; @B - Li; @Li3B14; @LiB3 ]. On the boron - rich side the experimentally reproducible compounds Li$_3$B$_{14}$ and LiB$_3 $ have large unit cells with fractional occupancies[@Li3B14; @LiB3; @PF ] and cannot be presently simulated with [ * ab initio * ] { } methods with desired degree of accuracy. The composition of the most lithium - fat LiB$_y$ compounds (near 50% concentration) obviously depend on deduction conditions and post - synthesis treatment, as the reported values for $ y$ range from 0.8 to 1 (notation explained in Ref. [ @xy ]). In the early experiments the form compounds were ascribed compositions Li$_5$B$_4$[@Wan78; @Wan79 ] or Li$_7$B$_6$[@Dal79 ]; Wang [ * at al. * ] { } used a rhombohedral model to explain the ascertained x - ray patterns[@Wan78; @Li5B4 ]. However, a more consistent interpretation of the available x - ray data on nearly stoichiometric lithium monoboride has been recently given by Liu [ * et al.*]{}[@aLi ]. The writer demonstrated that the main x - ray peaks can be index with a four - atom hexagonal unit cell $ \alpha$-LiB (Fig. 5(a) ), which consist of linear chains of boron embedded in hexagonal lithium shells[@aLi ]. 

 While the dim-witted $ \alpha$-LiB sheds sparkle on what the structure of the lithium monoboride is, an important doubt remains exposed as to
Ogufhi]. Consequently, we obsevve a noticeable increave in fhe relagive stability of the MS1 strnctuee foe higher-valent metals (kn fact, apl metal dibieides with at leasb fivs valznre electrons bekefit from hnsertion of at dxcra metal layer with the largest gaig of -340 mrV/wtom obtained sor GhF). Hosvvtr, these electron-rich systems allkw otheg phases with sigmificantly lower energies (orotltypes NiAs, NaCl, FfB-b, etc.[@PF]). Hghce, qe focus on uow-electron systems thzt have been shown to stabilize throbgh incorpotcrioj of extra mxtal lwyers and comkd com[ete wiyh existing phssev.

5. Lu-B system {#section.Li-B}
==============

[*Oterview.*]{} A few compougds at dixfzrent stoichiometries hqve bgen raporgwd wor tie Mi-B sydtej[@PF; @aLi; @bLj; @Alkali; @B-Lu; @Li3B14; @LiB3]. On the botog-goch side the experymqntally reproducible compounds Li$_3$B$_{14}$ and NiB$_3$ have large unit cells qith fractional occupwncies[@Li3B14; @LiB3; @PF] and cannot be presently simulated with [*ab initmo*]{} meuhids wkrh desired degree of accuracy. The composition os tne most lithium-rlch LiB$_y$ compounds (nfat 50% concentratiun) appcdehtly depends on syjthesis condutions anq poxt-synthesis treatment, as thw reported vcluws for $y$ range frol 0.8 to 1 (notacion ecplaimed in Ref. [@xy]). In the eaxly exleriments tje formed zompounds were arcrpbed composiukons Li$_5$B$_4$[@Wan78; @Wan79] ow Li$_7$B$_6$[@Dal79]; Xang [*ct al.*]{} usdd a rhombjhedral mofel to explain the obserged x-tay padterns[@Wan78; @Pi5B4]. However, a more consistent iiverpretation pf thv availabje x-rsy data on newrly stoichiomgtric litkium munoboride gas beei recently gyven by Liu [*ed al.*]{}[@aLi]. The anthors deionsrratwd that ghe main x-ray leaks can be indexee with a four-atom mexaguhal unit cell $\aophq$-LiB (Fig. 5(a)), whicn cunsysns pf ninear chainv of bofpn emcedded in hcxaeonak lithium shells[@aLi].

Wvile the simple $\alpha$-LoB sheds lught on rhat the struvture of the lithikm moioborive is, sn ymportant question remains opeh as to
Oguchi]. Consequently, we observe a noticeable increase relative of the structure for higher-valent diborides at least five electrons benefit from of an extra metal layer with largest gain of -340 meV/atom obtained for RhB). However, these electron-rich systems allow phases with significantly lower energies (prototypes NiAs, NaCl, FeB-b, etc.[@PF]). Hence, we focus low-electron that been to stabilize through incorporation of extra metal layers and could compete with existing phases. 5. Li-B {#section.Li-B} ============== [*Overview.*]{} A few compounds at different have been reported for Li-B system[@PF; @aLi; @bLi; @Alkali; @Li3B14; On the side experimentally compounds Li$_3$B$_{14}$ and have large unit cells with fractional occupancies[@Li3B14; @LiB3; @PF] and cannot be presently simulated with [*ab initio*]{} with desired accuracy. The of most LiB$_y$ compounds (near apparently depends on synthesis conditions and the reported values for $y$ range from 0.8 1 (notation in Ref. [@xy]). In the early the formed compounds were ascribed compositions Li$_5$B$_4$[@Wan78; @Wan79] Li$_7$B$_6$[@Dal79]; Wang [*at al.*]{} used a rhombohedral model to explain the observed x-ray patterns[@Wan78; @Li5B4]. more consistent interpretation of available x-ray data nearly lithium has recently given Liu [*et al.*]{}[@aLi]. The authors demonstrated that the main x-ray peaks be indexed with a four-atom hexagonal unit cell $\alpha$-LiB (Fig. consists linear chains of embedded in hexagonal lithium While simple $\alpha$-LiB sheds light the of is, important remains open as to
Oguchi]. Consequently, we obserVe a noticeaBle inCreAse In The rElatIve stability of THe MS1 Structure for higher-valeNt metAlS (In faCT, aLl metAl diborIDeS WIth At LeAst FiVE vAlencE elEctrons Benefit froM inSeRtion of an extRA mEtal layer wIth The largest gaIn oF -340 meV/atOm ObtAIned fOr RHB). HowEver, thESe elecTron-rich sYsTEms allOW other pHASeS witH significantly lowER eNErgies (prototypEs NiAs, nacL, FEb-B, etC.[@PF]). hence, we focUs On low-ELectron SYsTEMS thAT have been showN to stabilizE ThrOugh inCoRpoRAtion oF extrA mETal Layers and coUld cOmpete witH existINg phaseS.

5. li-B systEm {#sectIon.li-B}
==============

[*overVIeW.*]{} A Few CoMPouNDs At dIFfeRent stoiChIoMetriEs haVE BEEn rePorTed fOr the li-B system[@PF; @aLI; @bLI; @AlkALi; @B-li; @Li3B14; @liB3]. On The bOrOn-ricH side tHe expErImentally reprodUcibLe compounDs LI$_3$B$_{14}$ And lib$_3$ have LArge unIt cEllS with frActionaL OccUpANCIeS[@Li3B14; @LiB3; @PF] and cannot Be PREsEntly simUlated WItH [*aB Initio*]{} meThOds With DESired DegrEE oF accuracY. The coMPoSiTion of tHe Most liThIum-RicH LiB$_y$ COmpoUnds (neAr 50% concenTratiON) apparently depENds on synthesiS CoNDItIOns aNd pOst-synthesiS treATmenT, as tHE rEpoRTed vaLues fOr $Y$ RaNGe from 0.8 to 1 (notation expLaIned in ref. [@xy]). in the early expEriments thE FORmed compOundS WeRE ascribed compoSitioNs Li$_5$B$_4$[@Wan78; @WaN79] Or Li$_7$B$_6$[@Dal79]; wang [*aT al.*]{} used a RhombohedRAL model to ExpLaiN thE obSERvEd x-ray patternS[@wAn78; @Li5b4]. HOwever, a MorE consisTenT inTerPreTaTion of the AvailablE x-RaY dAtA on NearlY StoichioMeTriC lIthIum moNOboridE has bEen rEcEnTLy gIven by LIU [*eT AL.*]{}[@aLi]. thE aUthoRs dEmOnstrAted THat The main X-ray peaks Can BE indExEd With a foUr-atom hexagonAl Unit cell $\alPhA$-Lib (Fig. 5(a)), wHICh consisTs of linear chains of boron EMbedded In hExagoNal lIthium sheLls[@ALi].

WhiLe tHE simplE $\alpha$-liB shEdS liGHT on whAT ThE stRuCture of the LIThiUm monObOridE is, an imPortant question remAIns Open as to
Oguchi]. Consequently, weobserve anotic eab lein crea se i n the relative stab ility of the MS1 struc turefo r  hig h er -vale nt meta l s( i n f ac t,  al lm et al di bor ides wi th at leas t f iv e valence el e ct rons benef itfrom inserti onof anex tra metal  la yer w ith th e  large st gain o f- 340 me V /atom o b t ai nedfor RhB). However ,  t h ese electron-r ich sy st e ms a llo w o ther phase swiths ignific a nt l y low e r energies (p rototypes N i As,  NaCl,  F eB- b , etc. [@PF] ). Hen ce, we focu s on  low-elec tron s y stems t h at have  beensho wnto s t ab il ize  t h rou g hinc o rpo ration o fex tra m etal l a y ersand  cou ld co mpete with ex ist ingp has es.
5. Li -B s ys tem { #secti on.Li -B }
============= =

[ *Overview .*] {}  Afe w com p oundsatdif ferentstoichi o met ri e s ha ve been reported f or t he  Li-B sy stem[@ P F;  @ a Li; @bLi ;@Al kali ; @B-Li ; @L i 3B 14; @LiB 3]. On th eboron-r ic h side  t heexp erime n tall y repr oducible  comp o unds Li$_3$B$_ { 14}$ and LiB$ _ 3$ h av e  lar geunit cellswith frac tion a locc u panci es[@L i3 B 14 ;  @LiB3; @PF] and ca nn ot beprese ntly simulate d with [*a b i nitio*]{ } me t ho d s with desired  degr ee of accu r acy. The  comp ositionof the mo s t  lithium -ri chLiB $_y $ co mpounds (near 5 0% c on centrat ion ) appar ent lydep end son synthe sis cond it io ns  a ndpost- s ynthesis  t rea tm ent , ast he rep orted  val ue sf or$y$ ran g ef r om 0 .8  t o 1(no ta tionexpl a ine d in Re f. [@xy]) . I n  the  e ar ly expe riments the f or med compou nd s w ere as c r ibed com positions Li$_5$B$_4$[@ W an78; @ Wan 79] o r Li $_7$B$_6$ [@D al79];  Wa n g [*at  al.*] {} us ed  ar h omboh e d ra l m od el to expl a i n t he ob se rved  x-raypatterns[@Wan78; @ L i5B 4]. However,a m orec o ns ist e nt int er p ret a t ion of the avai lable x-ra yd at a on nearl y  st oi chiomet ric lit hiumm onobori de has be en recent ly  giv e n  by  Liu [*etal.*]{}[ @aLi]. Th e  auth o rs  demo nst ratedth atthe m ain x- r aypeaks  can b eindexe d wit ha four-a tom hexagonal unit cell  $\alp ha$-L iB(Fig. 5(a )), whi ch consis ts o f linear c hai nsof bo ron embed dedi nhex a gonal  lit h ium shell s [@ aLi ] . 
While the s i m p le$\alp ha$ - LiB sh edslight on what the structure of t he l i t hiu m m o nobo ri de is, an impo rta nt q uestionre mains openas to
Oguchi]. Consequently,_we observe_a noticeable increase in_the relative_stability_of the_MS1_structure for higher-valent_metals (in fact,_all metal diborides with_at least five_valence_electrons benefit from insertion of an extra metal layer with the largest gain of_-340_meV/atom obtained_for_RhB)._However, these electron-rich systems allow_other phases with significantly lower_energies (prototypes_NiAs, NaCl, FeB-b, etc.[@PF]). Hence, we focus on_low-electron_systems that have_been shown to stabilize through incorporation of extra metal_layers and could compete with existing_phases.

5. Li-B system_{#section.Li-B}
==============

[*Overview.*]{}_A_few compounds at different_stoichiometries have been reported for the_Li-B system[@PF; @aLi; @bLi; @Alkali; @B-Li;_@Li3B14; @LiB3]. On the boron-rich side the_experimentally reproducible compounds Li$_3$B$_{14}$ and LiB$_3$_have large unit cells with_fractional occupancies[@Li3B14;_@LiB3; @PF] and cannot be_presently simulated with_[*ab initio*]{}_methods with desired_degree of accuracy. The composition of_the most lithium-rich_LiB$_y$ compounds (near 50% concentration) apparently_depends_on synthesis conditions_and_post-synthesis_treatment, as_the reported values_for_$y$ range_from_0.8 to 1 (notation explained in_Ref._[@xy]). In the early experiments the formed_compounds were ascribed compositions_Li$_5$B$_4$[@Wan78;_@Wan79] or Li$_7$B$_6$[@Dal79]; Wang_[*at al.*]{} used a rhombohedral_model to explain the observed x-ray_patterns[@Wan78; @Li5B4]._However, a_more consistent interpretation of the available x-ray data on nearly stoichiometric_lithium monoboride has been recently given_by Liu [*et al.*]{}[@aLi]._The authors_demonstrated_that the main_x-ray_peaks can_be indexed with a four-atom hexagonal unit_cell $\alpha$-LiB_(Fig. 5(a)), which consists of linear_chains of boron embedded_in_hexagonal lithium shells[@aLi].

While the simple $\alpha$-LiB_sheds light on what the structure_of the lithium monoboride is,_an_important_question remains open as to